IPS e.max Ceram Scientific Documentation - ROE Dental Laboratory
Scientific Documentation IPS e.max ® Ceram Page 12 of 21 � IPS e.max Ceram is among the strongest veneering materials that can be used in combination with zirconium oxide. The biaxial flexural strength of this material by far surpasses the minimum value required by the relevant ISO standard. 3.3.3 Firing temperature Firing temperature [°C] 950 900 850 800 750 700 650 600 e.max Ceram Triceram Triceram Lava Lava Cercon Cercon S Nobel Nobel Zr Vita Vita VM9 VM9 Cerabien Cerabien Reihe1 750 755 810 830 910 910 930 Fig. 15: Firing temperatures of various veneering ceramics for use in conjunction with zirconium oxide (Ivoclar Vivadent AG Schaan, 2004/05) � IPS e.max Ceram demonstrates the lowest firing temperature of all the ceramic materials examined. Low firing temperatures reduce the processing times required for the fabrication of restorations.
Scientific Documentation IPS e.max ® Ceram Page 13 of 21 4. In vitro investigations 4.1 Fracture toughness of veneered bridges The fracture toughness was examined in veneered bridges without chewing simulation (after storage in water) and with chewing simulation. Eight samples were tested for each material and test method. The static tests were carried out in a universal testing machine. The load was applied directly to the pontic area. Those samples that included chewing simulation were placed in a chewing simulator and subjected to 1.2 million chewing cycles at a load of 50 N as well as to thermocycling at a temperature range of 5 °C/55 °C. Fracture load [N] 2500 2000 1500 1000 500 0 IPS e.max Press/ IPS e.max Ceram IPS e.max CAD/ IPS e.max Ceram IPS e.max CAD/ IPS Eris for E2 with chewing simulation without chewing simulation IPS e.max ZirCAD/ IPS e.max Ceram Fig. 16: Fracture toughness of veneered bridges with and without chewing simulation (Schröder/Spiegel, FH Osnabrück, 2005) 1 � The statistical analysis (Tukey) did not show any significant difference in the mean fracture load between the groups with and without chewing simulation. � The fracture load of bridges that consisted of IPS e.max ZirCAD (framework) and IPS e.max Ceram (veneering material) was significantly higher than that of all the other bridges examined. � The veneered bridges made of IPS e.max Press and IPS e.max CAD did not show any statistically relevant difference in terms of fracture load.